Active Standard ASTM D7227 / D7227M | Developed by Subcommittee: D04.21
Book of Standards Volume: 04.03
Historical (view previous versions of standard)
Significance and Use
3.1 Specimen dry weight is a critical measure in determination of accurate density and many other tests in the construction and raw materials industries. Drying specimens at room temperature is required for some tests and provides an advantage for other tests to ensure the integrity and to preserve the characteristics of specimens.
3.2 This practice covers drying compacted asphalt specimens in a vacuum chamber that is capable of keeping the specimen at close to room temperature. A vacuum pump reduces the pressure inside the chamber, thus allowing water to evaporate at low temperature. Since the specimen naturally cools during the evaporation process, making water harder to evaporate, it is important to have proper temperature controls in the chamber to ensure specimen remains at close to room temperature. Automatic controls within the unit allow the specimen to remain at close to room temperature by periodically allowing a flow of warm air to enter the vacuum chamber. Cycling between vacuum and airflow conditions allows the specimen to dry in a short period of time. Completely saturated specimens with over 30 g [0.07 lb] of retained water can be dried in about 30 minutes. For most field cores that are not completely saturated the drying time is generally less than 15 minutes.
3.4 This method can also be used for drying loose asphalt mixtures, aggregate samples and other solid specimens. Follow manufacturers recommended procedures for drying specimens other than compacted bituminous specimens.
1.4 This practice can also be used for drying other construction materials such as concrete, soils, aggregates and loose asphalt mixtures. Use manufacturers recommendations for drying other construction materials.
1.5 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalent; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D5361 Practice for Sampling Compacted Bituminous Mixtures for Laboratory Testing
ICS Number Code 91.100.50 (Binders. Sealing materials)